Developing Novel Platinum Group Metal-Free Catalysts for ......Developing Novel Platinum Group Metal...
Developing Novel Platinum Group Metal-Free Catalysts for Alkaline Hydrogen and Oxygen Evolution Reactions (DE-EE0008082) PI: Prof. Sanjeev Mukerjee Department of Chemistry and Chemical Biology, Northeastern University 360 Huntington Ave, Boston, MA 02115 June 13 th , 2018 Project ID#: pd156 2018 DOE Hydrogen and Fuel Cells Program Review This presentation does not contain any proprietary, confidential, or otherwise restricted information
Developing Novel Platinum Group Metal-Free Catalysts for ......Developing Novel Platinum Group Metal -Free Catalysts for Alkaline Hydrogen and Oxygen Evolution Reactions(DE-EE0008082)
Text of Developing Novel Platinum Group Metal-Free Catalysts for ......Developing Novel Platinum Group Metal...
Developing Novel Platinum Group Metal-Free Catalysts for Alkaline Hydrogen and Oxygen
PI: Prof. Sanjeev MukerjeeDepartment of Chemistry and Chemical Biology,
Northeastern University360 Huntington Ave, Boston, MA 02115
June 13th, 2018Project ID#: pd156
2018 DOE Hydrogen and Fuel Cells Program Review
This presentation does not contain any proprietary, confidential, or otherwise restricted information
Project PartnersPI: Sanjeev Mukerjee - Northeastern UniversityPartner organizations:• University of Delaware – Prof. Yushan Yan• Advent North America – Dr. Emory De Castro
This project will develop stable, high-conductivity, and high-strength AEMs, stable and active PGM-free catalysts for hydrogen and oxygen evolution reaction (HER/OER), and high-performance electrode architectures.
The materials being developed under this project have the potential to unlock the cost advantages of AEM electrolyzers, enabling a clear pathway for achieving <$2/KgH2 (on scale) with efficiency of 43 kWh/kg H2 via anion exchange membrane (AEM)-based electrolysis.
Award # EE0008082
Start DateYear 1 End DateProject End Date
Total DOE ShareTotal Cost ShareYear 1 DOE Funding
Approach - Summary
BarriersCurrent state-of-the-industry anionic exchange membranes are subject to degradation above 60 OC. This project aims to develop a new anionic exchange membrane capable of operating at elevated to temperatures, thereby increasing the kinetics of electrolysis.
Key MetricsUnits Baseline Year 1
Cell voltage V 2 1.92
Current density A/cm2 0.5 0.8
Operating temp OC 80 80
Membrane ASR Ω cm2 .13/.08 0.15
HER volumetric + overvoltage @500 mA/cm2, 25 OC
OER volumetric activity @1.47VRHE, and overvoltage @500 mA/cm2, 25 OC
Model voltage V 1.65 1.74
Unexplained voltage loss
V 0.35 0.18
The focus of this project is on durable, high-performance materials advanced water splitting,enabling a pathway for achieving <$2/KgH2 withefficiency of 43 kWh/kg H2 via anion exchangemembrane (AEM)-based electrolysis. We aim toadvance these goals via an understanding of bothhydrogen and oxygen evolution reactions leading tonovel platinum group metal (PGM)-free catalystmaterials in conjunction with improvements inmembrane and ionomers and gas evolutionelectrodes with corresponding characterization andtesting.
– Northeastern Univ., (Prime) Boston, MA: S. Mukerjee (P.I):• Novel HER catalysts:
• Metal-Metal Oxides• Functionalized mono-metallic• Embedded Metal-N-C Systems
• Novel OER Catalysts: • Double layer metal oxides on Raney Ni (strategies for increasing active site
density)• Half and Single Cell Tests (NEU)• In situ Raman and Synchrotron X-ray Spectroscopy
– University of Delaware (Sub-awardee), Newark, DE: Prof. Y. Yan• Novel Membranes and Ionomers
• Design of multi-cation Poly(aryl-piperidinium) Tri-quaternary-ammonium (PAP-TQN) membranes and ionomers for high temperature operation (90oC).
– Advent North America (Sub-awardee), Cambridge, MA: Dr. Emory De Castro• Novel Electrodes designed for gas evolution with and without liquid flow
– National Lab Partners:• NREL – MEA Prep and testing• LBNL – Small Angle Scattering and Transport Modeling• Sandia National Labs – Interfacial modeling
Partnerships and Roles
Approach - Summary
Relevance and Impact
• This program aims to develop thermally sustainable anionic membranes that will enable the use of cost-efficient transition metal catalysts.
• Our group will be able to leverage the capabilities of the ENM to generate multiscale modeling and molecular dynamics generated simulations of the membrane catalyst interface. In addition, its expertise with advanced ionomer materials, the EMN will provide durability and validation protocols of electrolyzer materials
• These activities can be applied to other areas of electrolysis research to characterize ionomer stability and electrolyte ion flux.
Approach – HER in Alkaline
Volmer:M + H2O + e- → M-Hads + OH-
M-Hads + H2O + e- → H2 + OH-
Tafel: 2 Pt-Hads → H2
Poor catalysts: θH << 1
Volmer (rds) - Tafel
Good catalysts:θH ~ 1
Volmer –Heyrovsky (rds)
Strategy 1: State of the art Metal-Metal Oxide electrocatalysts
Approach - Materials Design Strategy: Non-PGM HER Electrocatalysts
Milestone Summary TableRecipient Name: Northeastern University
Project Title: Enabling Efficient Water Splitting with Advanced Materials Designed for High pH Membrane Interface
Task orSubtask (if applicable)
(Milestone or Go/No-Go Decision
Milestone Description(Go/No-Go Decision Criteria)
(Quarters from Start of the
1.1 Milestone M1.1: Deliver three 5 gm batch samples of Ni-MOx/C HER catalysts for RDE and Single Cell tests with η of 300 mV @ 500 mA/cm2 and 2 A/cm3 (HER)
Completed1.2 Milestone M1.2: Deliver one 5 gm batch of Ni-Nx/C HER catalysts for RDE and Single cell studies η of 300 mV
@ 500 mA/cm2 and 2 A/cm3 (HER)Q2
1.3 Milestone M1.3: Deliver one 5 gm batch of M-N(S)-C MOF HER catalysts for RDE and Single cell studies η of 300 mV @ 500 mA/cm2 and 2 A/cm3 (HER)
1.4 Milestone M1.4: Deliver three 5 gm batches of MMOx OER catalysts for RDE and single cell tests Q2100%
Task 2 2.3 Milestone M2.3: Deliver at least 5 grams of PAP-TQN ionomers and cast membranes that have less than 20% loss of IEC in 1 M KOH at 90 °C for 100 hours (Q3).
BP1 Go/No Go Decision Point
HER Electrocatalysts: Using PGM-free HER electrocatalsyts in an AEM MEA operating under electrolysis conditions, at a current density of 500 mA/cm2 achieve 300 mV or lower overvoltage and volumetric current density (VCD) of 2 A/cm3 .OER Electrocatalysts: Using PGM-free OER electrocatalsyts in an AEM MEA operating under electrolysis conditions, at a current density of 500 mA/cm2 achieve 150 mV or lower over-voltage and 6 A/cm3 (VCD).AEM Membranes and Ionomers: Achieve AEM membrane ASR of 0.15 Ω cm2 measured in MEA and less than 20% loss of IEC in 1 M KOH at 95°C for 1000 hours. AEM MEA: Demonstrate PGM-free AEM MEA electrolyzer performance of 0.8 A/cm2 at ≤1.92 V .
Main Takeaways • Ni-MOx outperforms Pt as HER catalyst • UDel PAP-TP-Me membrane is stable at high temperatures
• Ni-Nx is a viable alternative to Pt as an HER catalyst
H2 Pump Cell• H2 pump experiments measure the
HER activity directly by decoupling the overall cell potential from OER.
• Ni-cup/C exceeds the Q1 milestone of 300mV at 500mA/cm2
• Ni-cup/C out performs Pt by 400 mV at 500 mA/cm2.
• UDel membrane out performs A201 in a Pt/C H2 pump
H2 Pump - Polarization Curve
H2 Pump - Polarization Curve
Anode: Pt/CCathode: Pt/C
• Metal / Metal-oxides weaken H-OH bond in H2O to facilitate Volmer reaction
Enhance formation of M-Hadsintermediate
• Metal / Metal-oxides benefit from enhanced HER in presence of AEI
Poisoning adsorbate for PGM catalysts
• Further optimization of M/M-Ox surfacesComposition & Morphology
• K2CO3 at the cathode poisons the membrane via electro-osmotic drag.
• Large amounts of water at either electrode floods the electrode and reduces performance.
• Water is delivered to “dry” anodes via water molecules solvating the OH- crossing the membrane.
• Water is delivered to dry cathodes by back diffusion of water.
• The best results are obtained with K2CO3 solution at the anode.
Electrolysis cell performance trends
Water Splitting: Non-PGM Testing
• OER catalyst: 3.08 mg/cm2 NiFe/Raney• HER catalyst: 2.94 mg/cm2 Ni-cup/C• Operating temperature: 90 OC• Anolyte: 1% K2CO3 at 300mL/min• Membrane: Baseline: Udel PAP-TN
BP 1 Target• 1.92 V, 800C, 800 mA/cm2
Quarter Task 2: Preparation of PAP-TQN polymer
Q1-4 Subtask 2.1: Synthesis of PAP-TN polymers
PAP-TN is synthesized by polyhydroxyalkylation of N-methyl-4-piperidone, trifluoro-acetophenone and terphenyl. Reaction and polymerization conditions, i.e., temperature, solvent and reaction time, will be optimized.
Subtask 2.2: Synthesis of two-ammonium-cations iodo-alky side-chain (DQN-I)
DQN-I is synthesized in two steps by Menshutkinreactions between a diamine, methyl iodide, and 1,6-diiodohexane. Reaction conditions, i.e., reactant ratios, temperature, solvent and reaction time, will be optimized.
Subtask 2.3: Synthesis of PAP-TQN polymers
PAP-TQN is synthesized by Menshutkin reaction of PAP-TN and DQN-I. Reaction conditions, i.e., temperature, solvent and reaction time, will be optimized.
Milestone 2.3: Deliver 5 grams of PAP-TQN ionomers and cast membranes that have less than 20% loss of IEC in 1 M KOH at 90 °C for 100 hours (Q3).
Subtask 2.4: Preparation and evaluation of PAP-TQN membrane
Reliable procedures of membrane; Screening of solvent, co-solvent, temp. and casting condition; evaluation of IEC, OH- conductivity, water uptake, mechanical properties, alkaline stability, gas permeation and microstructure
Go/No Go Decision: Achieve AEM membrane ASR of 0.15 Ω cm2 measured in MEA and less than 20% loss of IEC in 1 M KOH at 95°C for 1000 hours.
Mechanical properties: Strain at break = 9% (elongation), Stress at break = 160 Mpa
(X = I, room temperature, average number)
IEC (ion exchange capacity) = 2.00 mmol/g (X = OH, theoretical)Crystallinity: will be measured with wide angle x-ray scattering
Accomplishments - Membrane Properties
Collaboration: Effectiveness• Models provided by Sandia National Labs have shed light on the response of
the ionomer active site to charge. Specifically, the distance between cationic sites and solvation of the anion were examined. This study will be useful to determine the optimal side-chain length and ion-exchange capacity of future ionomer materials.
• Small angle X-ray scattering studies were performed at LBNL to gain insight on the morphology of the anion exchange membrane in different states of hydration.
• LBNL has also modeled the interaction of carbonate ions at the interface of the catalyst layer and the anion exchange membrane. The model has provided insight into how and where the ion accumulates in an electrolysis cell when different amounts of current are applied.
• Modeling of the ionomer structure at the interface has begun and is showing the effect of metal charge and its effect on the ionomer morphology
• The efforts of our EMN partners are described in detail in the Technical Back-Up Slides
Proposed Future Work
1. Materials Discovery: (NEU & Udel) FY2 (Q1-Q4)• HER Catalysts: Ni-Nx catalyst optimization, stability tests, structure function
determination. Preparation of MOF derived catalysts.• OER catalyst: Enhance active site density of Ni-Fe-Co/Raney Ni• Membrane and Ionomer: Extensive durability tests, Full Cell Testing at
elevated temperatures• Electrodes and Ink Composition: New electrode design with novel ink
compositions2. Cell Tests: (NEU) FY2 (Q2-Q4)
• Accurate determination of OER overvoltage• Optimization of Full Cell for long duration tests
3. In situ XAS and Raman Measurements: (NEU): FY2 (Q2-Q3)4. Detailed modeling of transport processes for deciphering carbonate effect
(LBNL) FY2 (Q2)5. SAXS measurement for membrane structure and morphology as a function of
temperature, ion exchange and humidity (LBNL) FY2 (Q2-Q4)6. Interfacial modeling to understand ionomer effects (Sandia) FY2 (Q2-Q4)7. Durability measurements on PAP-TQN membranes (NREL) FY2 (Q3-Q4)8. MEA optimization and testing (NREL) FY2 (Q3-Q4)
Technical Backup Slides
HydroGEN Advanced Water Splitting Materials 23
SAXS Measurements-LBNL (A Kusoglu)
• Key findings 2D Scattering Spectra (images, not shown here)
indicates isotropic structure No preferential orientation There is weak degree of phase-separation Very broad, less apparent peak Not a significant difference among the 4 samples
tested Structure does not appear to change much from
ambient to liquid (full hydration) state The polymer exhibits a more or less a “gel”-like or
Interpretation and future Efforts– Need to correlate this with the water uptake
capacity of the samples• How much water does the membrane uptake from
dry to liquid state?– Spectroscopic analysis to help interpret the
morphology from SAXS– Possible effects of carbonate formation?• May need to prepare samples for SAXS in
controlled environment– Next experiment:• Controlled heating in liquid water
LAWRENCE BERKELEY NATIONAL LABORATORY | ENERGY TECHNOLOGIES AREA
• System appears more tolerant of CO3
2- in anode than in cathode.• HFR suggests CO3
2- at cathode interferes with self-purging.
• CO32- desorption as CO2 (g) isn’t
fast enough to clear away CO32-
introduced at cathode.
Effects of carbonate in AEM electrolyzers
None (OH- form)
𝑦𝑦𝐶𝐶𝑂𝑂32− = 0.9 at listed boundary
AEM CLCL GDLGDL1-D cell model
Set CO32- fraction
𝑦𝑦𝐶𝐶𝑂𝑂32− = 0.9Allow CO3
2- flux (solid lines)No CO3
2- flux (dashed)
LAWRENCE BERKELEY NATIONAL LABORATORY | ENERGY TECHNOLOGIES AREA
Carbonate distribution in MEA
• Carbonate accumulates in anode in all cases
• Lack of CO32- in cathode feed
allows OH- production to clear out CO3
2- in membrane• Next steps:Modeling of ion-exchange process
between membrane and liquid electrolyte
Incorporate additional carbonate effects on HER/OER kinetics as observed by NU
Explore sensitivity to material properties to identify performance limitations
𝑦𝑦 𝐶𝐶𝑂𝑂 32−
𝑦𝑦 𝐶𝐶𝑂𝑂 32−
𝑦𝑦 𝐶𝐶𝑂𝑂 32−
𝑦𝑦 𝐶𝐶𝑂𝑂 32−
accumulation at high current
Structure response to electrode charge4 ionomer chains of length: 100 units, with water and OH interacting with a metal surface In this preliminary data we see
• The N+ charge centers are attracted by negatively charged metal surface and greatly repelled by positively charged metal surface
• The N:N distance peaks at ~9A and the peak increases with positive charge, which implies compaction of the ionomer chains
• The average number of OH solvating the N charge centers on the ionomer chains increase with positive surface charge
Water omitted for clarity
Interfacial Modeling: Sandia (Reese Jones)
Current and Future Work• Obtain experimental mass density and use this and the water percentage to build system with the correct
species concentrations• Investigate the structure plausibility of the resulting systems• Add H+ (and compensating OH-) to explore pH effects on the structural response to metal surface charge.Ultimately, use representative subconfigurations to investigate charge transfer with ab initio methods